Fracture Mechanics of Composites with Residual Thermal Stresses


 Frank Young
 2 years ago
 Views:
Transcription
1 J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate for crack growth in an arbitrary composite in the presence of residual stresses is considered. First, a general expression is given for arbitrary, mixed traction and displacement boundary conditions. This general result is then applied to a series of specific problems including statistically homogeneous composites under traction or displacement boundary conditions, delamination of double cantilever beam specimens, and microcracking in the transverse plies of laminates. In many examples, the energy release rate in the presence of residual stresses can be reduced to finding the effect of damage on the effective mechanical properties of the composite. Because these effective properties can be evaluated by isothermal stress analysis, the effect of residual stresses on the energy release rate can be evaluated without recourse to any thermal elasticity stress analyses. Introduction When a composite comprised of materials having disparate thermal expansion coefficients is subjected to a uniform change in temperature, it will develop residual thermal stresses. If that composite develops cracks, either as a result of the residual thermal stresses or of some subsequently applied mechanical tractions, the residual and mechanical stresses will change to accommodate the fracture surfaces. One effect of the redistribution of residual thermal stresses is a change in the effective thermal expansion coefficient of the composite Hashin, 988. Additionally, the redistribution of residual and mechanical stresses releases strain energy that can drive crack propagation the energy release rate for crack growth. The goal of this paper is to evaluate the effect of residual thermal stresses on the energy release rate for crack growth in composites. The redistribution of residual and mechanical stresses caused by cracks can be viewed as similar elasticity problems but with different boundary conditions. Because of their similarity, it is often possible to explicitly account for the effect of residual thermal stresses without doing a thermal elasticity analysis of the composite. Some general energy release rate expressions including residual thermal stresses are derived in the first section of this paper. The general results are for an arbitrary composite under arbitrary, mixed traction and displacement boundary conditions. Next, the general expressions are applied to statistically homogeneous composites, double cantilever beam delamination specimens, and microcracked laminates. The simplest possible energy release rate expressions are derived. In some examples, the energy release depends on knowledge of both the mechanical and residual stress states, but, in some important practical examples, the energy release rate can be expressed in terms of the effect of cracks on the effective composite mechanical properties. These effective mechanical properties can be derived using elasticity analyses that ignore residual stresses. General Theory Consider an arbitrary, multiphase composite subjected a uniform temperature change of T = T and to any mixed traction and displacement boundary conditions. Let the surface be S = S T S u, where S T is that part of the surface subjected to traction boundary conditions: T = T 0 = σ 0ˆn where σ 0 is the surface applied stress note: all tensors are written in boldface and ˆn is a unit normal to the surface. S u is that part of the surface subjected to displacement boundary conditions: u = u 0 = ε 0 x 804 / ol. 64, DECEMBER 997 Transactions of the ASME
2 where ε 0 is the surface strain and x is a position vector on the surface. T 0 and u 0 are the boundary conditions; in general they may depend on position. Note also that tractions and displacements may be applied over the same portions of the surface provided they are applied along different coordinates. For example, one section of the surface may have traction in the x direction but fixed displacement in the y direction. Similar to Rosen and Hashin 970, the full thermal elasticity problem can be treated as a superposition of two problems. First, let σ m and ε m, with tractions T m and displacements u m, be the solution to the isothermal T = 0 elasticity problem: σ mˆn = T 0 on S T 3 u m = u 0 on S u 4 σ m = Cε m and ε m = Sσ m 5 where C and S are the stiffness and compliance tensors. In a composite, C and S will depend on position. As the solution to an elasticity problem, σ m satisfies equilibrium and ε m satisfies compatibility. Second, let σ r and ε r, with tractions T r and displacements u r, be the solution to the thermal elasticity problem: σ rˆn = 0 on S T 6 u r = 0 on S u 7 σ r = Cε r αt and ε r = Sσ r + αt 8 where α is the positiondependent thermal expansion tensor, σ r satisfies equilibrium, and ε r satisfies compatibility. Note that T r may be nonzero on S u and u r may be nonzero on S T. A superposition of the above two solutions, σ = σ m + σ r and ε = ε m + ε r, solves the complete thermal elasticity problem σ ˆn = T 0 on S T 9 u = u 0 on S u 0 σ = Cε αt and ε = Sσ + αt σ m and ε m are the mechanical stresses and strains while σ r and ε r are the residual thermal stresses and strains. The internal energy is the volume integral of stress dotted into strain relative to the freeexpansion strains. This energy can be expressed in terms of mechanical and residual stresses: U = σ ε αt d = σ m Sσ m d + σ m Sσ r d + σ r Sσ r d Assuming tractionfree crack surfaces and using the divergence theorem, the mechanical stress term in Eq. may be written in terms of mechanical surface tractions, T m, and displacements, u m, as σ m Sσ m d = T 0 u m ds + T m u 0 ds 3 S T S u T 0 u r ds 4 For the cross term in Eq., the displacements caused by the residual thermal stresses can be considered as virtual displacements to the mechanical strains or δ u = u r. They correctly have u r = 0 on S u. By virtual work σ m ε r d = S T But also, ε r = Sσ r + αt, giving σ m Sσ r d = T 0 u r ds σ m αt d 5 S T Analogously, the residual tractions, T r, can be considered as virtual forces on the mechanical stresses; σ r obeys equilibrium and T r = 0 on S T. Thus, again by virtual work ε m σ r d = σ m Sσ r d = T r u 0 ds 6 S u Journal of Applied Mechanics ol. 64, DECEMBER 997 / 805
3 Finally, for the pure residual stress term in Eq. : σ r Sσ r d = σ r ε r σ r αt d = S T r u r ds σ r αt d 7 But, over the entire surface, either T r = 0 or u r = 0, giving σ r Sσ r d = σ r αt d 8 Combining Eqs. 3, 5, 6, and 8 gives U = T 0 u m ds + T m u 0 ds + T r u 0 ds σ r αt d 9 S T S u S u σ m αt = T 0 u r ds T r u 0 ds 0 S u S T For fracture mechanics analysis we need to evaluate the energy release rate defined as G = dw du where W is external work and A is fracture area. The external work is caused by the action of the mechanical tractions on S T applied over the total displacements. Thus dw = d T 0 u m + u r ds Combining this result with Eqs. 9 and 0 gives G = G mech + T S T d σm α + d σr α where G mech is the mechanical energy release rate or the energy release when T = 0: G mech = d T 0 u m ds T m u 0 ds S T and angle brackets indicates a volumeaveraged quantity: fx, y, z = fx, y, zd 5 Note that the full, thermodynamic internal energy in thermal elasticity includes heat capacity terms. The energy associated with residual stresses that exist under zero traction or zero displacement, can be viewed as contributing to the effective constant pressure or constant volume heat capacity of the composite Rosen and Hashin, 970. Here the residual stress energy contributes to the total energy release rate for crack growth. The heat capacity terms associated with individual phases, however, can be ignored when calculating energy release rates because they drop out when the derivative with respect to crack area is evaluated. The result in Eq. 3 includes nothing specific about composites. The result for a composite with n phases is G = G mech + T v i α i S u dσim + dσir where superscript i means a property of phase i, v i is the volume fraction of phase i, and the over bar indicates a phaseaveraged quantity integrated over the volume of phase i, i : σ im = σ m d 7 v i i 806 / ol. 64, DECEMBER 997 Transactions of the ASME 3 4 6
4 In deriving Eq. 6, it was assumed that the component thermal expansion tensors in each phase are independent of position within that phase. This situation always holds for composites with isotropic phases. For composites with anisotropic phases at variable orientations, each orientation must be considered as a separate phase for analysis by Eq. 6. When anisotropic phases are aligned, such as in unidirectional, carbonfiber reinforced composites, the anisotropic phase can be considered as a single phase. Although the general result in Eq. 6 depends on both mechanical and thermal stresses, in some important special cases, the energy release rate can be expressed solely in terms of mechanical properties and stresses. For example, in many fracture situations, cracks will propagate such that failure is by pure mode I fracture or pure opening mode fracture. For example, it has been suggested that regardless of external loading conditions that delamination always proceeds by mode I fracture Charalambides et al., 99. Under pure mode I crack growth, energy release rate is related to mode I stress intensity factor by G I K I 8 In linear thermal elasticity, K I must be linearly related to applied load and temperature change. If we thus consider uniformly scaling all applied tractions and displacements to be where P is a scalar multiplier, stress intensity must have the form T app = P T 0 and u app = P u 0 9 K I = c P + c T 30 where c and c are some constants that depend on material properties and geometry of the crack. The energy release rate must therefore have the form Comparing Eq. 3 to Eq. 6 we can prove that G I c P + c T 3 T Substitution back into Eq. 6 gives v iα i dσim = v iα i dσir G mech v iα i dσim G I = + T G mech v iα i dσim G mech 3 33 Remarkably, the energy release rate including residual thermal stresses depends only on the results from a mechanical stress analysis. Thus, the effect of residual stresses can be determined without any need for solving a thermal elasticity problem. Although this result was derived for pure mode I crack growth, analogous expressions hold for pure mode II or III crack growth. Examples Uniform Traction, Statistically Isotropic Composite A useful model for evaluating effective properties of composite materials is to consider a statistically homogeneous composite Hashin, 963; 969. Such composites are analyzed by averaging over a representative volume element; this element must be chosen large enough to have all averaged results representative of the averaged results for entire composite Hashin, 963; 969. Here we also consider the representative volume element to have cracks that are representative of the entire composite. Such a representative volume element is then subjected to a uniform traction or a traction that arises from a surface stress, σ 0, that is independent Journal of Applied Mechanics ol. 64, DECEMBER 997 / 807
5 of position. By the average strain theorem Hill, 963; Hashin 963; 969, the only remaining integral in G mech reduces to T 0 u m ds = S σ0 ε m D m = σ0 S σ 0 34 where S is the effective compliance tensor of the composite Hashin, 963; 969. The tensor D m is related to the crack opening mechanical displacements and is defined by Dij m = u m j n i + u m i n j ds i, j = x, y, or z 35 S c where S c is total crack surface area. The effective composite compliance is defined in terms of the apparent average strain which is the bulk average strain reduced by the crackopening tensor Aboudi, 994; thus S σ 0 = ε m D m 36 Substituting Eq. 34 into Eq. 6 the energy release rate becomes G = σ 0 ds σ0 + T v i α i dσim For pure mode I or II, or III crack growth the energy release rate becomes G I G mech = + T v iα i dσim σ 0 ds σ0 ] + dσir Finally, for a two phase composite a composite with two isotropic phases or two aligned anisotropic phases we have S v dσ m dσ v m + v dσ m + S v dσ m = 0 39 = d εm = ds σ0 + ddm For pure mode fracture we can derive ] σ G I = 0 + T α α S S ds σ0 + T α α S S ddm 4 σ 0 ds σ0 The energy release rate depends only on the effective compliance tensor and the mechanicallyinduced crackopening displacement tensor. Note the D m only affects the energy release rate when there are residual thermal stresses; in the absence of residual stresses, G I depends only on S. Uniform Displacement, Statistically Isotropic Composite For uniform displacement u 0 = ε 0 x where ε 0 is independent of position applied to a statistically homogeneous composite, use of the average stress theorem leads to G mech = d σ m 40 ε0 = ε0 dc ε0 4 where C is the effective stiffness tensor of the composite. For a better analogy with the uniform traction results, some terms can be reexpressed as: α i σ im = M i ε im 43 α i σ ir = M i ε ir + α i M i T / ol. 64, DECEMBER 997 Transactions of the ASME
6 P u y x u P Fig. A double cantilever beam specimen using unidirectional composites. The fiber direction indicated by the internal lines is parallel to the delamination crack growth. The specimen is point loaded by loads of P. The total deflection between the loading points is u. where M = Cα is the stresstemperature tensor. Incorporating these results into the Eq. 6 and ignoring the constant term α i M i T, which drops out upon differentiation, the energy release rate is ] G = ε 0 dc ε0 + T v i M i dεim + dεir 45 This result is identical to the uniform traction results see Eq. 37 except for a sign change and physical meanings of all symbols. The sign change is required because G is positive and, in general, C decreases with crack growth. By an explicit analogy to the results for uniform traction, the energy release rate for pure mode crack growth becomes Delamination G I G mech = + T v im i dεim ε 0 dc ε0 Figure shows a double cantilever beam specimen made from a unidirectional composite. The fibers run parallel to the x direction. This problem differs from the previous sections in two respects. First, the specimen is not statistically homogeneous because there is only one macroscopic delamination crack. Second, although there is only traction loading, the tractions are not uniform i.e., they depend on position. The tractions can be written as T 0 = P δ x x upper δ x x lower ] 47 where δ x is the Dirac delta function and x upper and x lower are the locations of the upper and lower load points. Substitution into Eqs. 4 and 33 because the crack growth is pure mode I gives v iα i dσim G I = P dc m + T P dc m where C m = u m /P is the mechanical loadpoint compliance. The leading term is G mech or the energy release rate in the absence of residual stresses Proceeding for a twophase unidirectional composite fibers as phase and matrix as phase with aligned transversely isotropic phases, we can write v i α i dσim = v σ xx m α A + σ yy m + σ m zz ] α T + v σ xx m α A + σ yy m + σ m zz ] α T Journal of Applied Mechanics ol. 64, DECEMBER 997 /
7 σ 0 σ 0 x 90 Plies t z s n B σ 0 σ 0 Fig. An edge view of a microcracked laminate. The microcracks occur in the central 90 plies; they are located at the top and bottom of the 90 plies are are separated by a distance s. Each ply has thickness t i ; the total symmetric laminate thickness is B. Now, doublecantilever beams specimens without residual stresses can be well analyzed using beam analyses Hashemi et al., 990. Within the assumptions of a beam analysis σ yy im and σ zz im are identically zero while σ xx im will net to zero by virtue of a balance between tension and compression stresses within the beam. The energy release rate for delamination becomes simply G = P dc m 50 In other words, within the assumptions of beam analyses, residual stresses have no effect on delamination. Residual stresses are present in both the fiber and the matrix, but they release no energy as the delamination propagates. Microcracked Laminate Figure shows an edge view of a symmetric, nply laminate under a uniaxial load of σ 0 in the x direction in which the central 90 ply group has throughthewidth cracks separated by a distance s. This geometry is appropriate for analysis of a microcracked laminate with periodic microcracks in the 90 plies having a density D = /s Nairn and Hu, 994. This problem differs from previous examples in three respects. First, the tractions are nonuniform: σ 0 is applied to the uncracked plies, but there is zero traction on the cracked 90 plies. Second, there are more then two phases. Although the plies themselves are composites, here each ply is treated as a homogeneous, anisotropic material. The general laminate, which may have plies at many orientations or may even be a hybrid laminate, is thus a multiphase composite. Third, we incorporate information about the laminated structure of the composite into the analysis. The key structural information we use is that the x and y direction strains of all uncracked plies are equal and that σ zz im plies. From Eq. 3, we can immediately write G = = σ ir zz = 0 in all d σ 0 + T σ m α + σ r α 5 80 / ol. 64, DECEMBER 997 Transactions of the ASME
8 where E xx is the effective laminate modulus in the x direction. The first term is the energy release rate in the absence of residual stresses. Furthermore, by Eq. 0 we can write σ m αt = σ 0 ε r xx u = σ 0 α xxt 5 where αxx is the effective laminate thermal expansion coefficient in the x direction and ε r xx u is the volume averaged residual strain in the uncracked plies only. This term appears because the tractions are applied only to the uncracked plies. Equation 5 is similar to Levin s analysis for thermal expansion coefficient of a composite Levin, 967; Rosen and Hashin, 970 except that it is applied here under conditions of nonuniform traction. The energy release rate will be analyzed first using a plane stress analysis in which σ yy im all plies. From Eq. 5: σ 0 α xx = = σ ir yy = 0 in v i σ xx im α xx i 53 where v i = t i /B is the total volume fraction of ply i including both sides of the symmetric laminate. By force balance and isostrain in the uncracked plies v i σ xx im = σ 0 and σ xx im = Ei xxσ 0 for i 54 Using these results, the effective xdirection thermal expansion coefficient can be expressed as αxx = α xx i v α xx E xx u E xx 55 where α xx = α xx α u xx, E xx u i= = v ie xx i, and α u i= xx = v iα i v n i= v ie xx i xxe xx i E xx u and α xx u are the ruleofmixtures xdirection modulus and thermal expansion coefficient of the uncracked plies. The residual strain energy term is σ r αt = By force balance of residual stresses and isostrain in the uncracked plies v i σ xx ir = o and σ xx ir Using these results, the residual strain energy term is 56 v i σ ir xx α i xxt 57 = E xx i α xx α i xx T for i 58 σ r αt = constant α xx v T α xx E u xx 59 The constant term is not evaluated because it drops out when finding the energy release rate. Substituting Eqs. 5, 55, and 59 into Eq. 5 gives G = d σ 0 α xx E xx u v T E xx 60 The energy release rate in the presence of residual thermal stresses depends only on one effective property E xx; that property can be evaluated by an isothermal stress analysis. If we imagine formation of a complete new microcrack midway between two existing microcracks, we have = BW s = BW D and = t W = v BW 6 Journal of Applied Mechanics ol. 64, DECEMBER 997 / 8
9 The integrated energy release rate for formation of a complete microcrack is G = σ 0 α xx E xx u v T v D 6 where /E xx is the change in the effective xdirection modulus caused by the new microcrack. An energy release expression mathematically identical to Eq. 6 is given in a different form in Nairn et al. 993 and Nairn and Hu 994 and in the identical form in Nairn 995. In Nairn et al. 993, Nairn and Hu 994, and Nairn 995, however, the energy release rate was the specific result of a thermal elasticity analysis. Here the energy release rate is derived as a general result. The accuracy of finding G is only limited to the accuracy in finding E xx. In Nairn 995, variational mechanics was used to bound E xx and an average of those bounds gave a virtually exact solution for G. A better connection with laminated plate theory can be derived by considering a generalized planestrain analysis of a cracked laminate instead of the previous plane stress analysis. In the generalized planestrain analysis, it is assumed that the ydirection strain in all plies is ν xyσ 0 /E xx where ν xy is the effective xy Poisson s ratio of the cracked laminate. The resulting new analysis will correct the plane stress analysis to account for differential Poisson s ratios between the plies. The corrections are generally small, but can be accomplished in a straightforward analysis. Equations 5 and 5 are unchanged in the generalized planestrain analysis. Starting from Eq. 5: σ 0 α xx = v i σ xx im xx + v i σ yy im α yy i α i 63 By force balance and isostrain in the uncracked plies v i σ im xx = σ 0 and σ im xx = Q i ν xyq i σ0 σ yy im = Q i ν xyq i σ0 E xx v i σ im yy = 0 64 for i 65 for i 66 where Q i kj k, j =,, 6 are the suitablyrotated elements of the inplane stiffness matrix for ply i Tsai, 987. Using these results, the effective xdirection thermal expansion coefficient becomes α xx = α xx + E xx i= ν xy E xx ] v i α xx i α xx Q i + α yy i α yy Q i i= ] v i α xx i α xx Q i + α yy i α yy Q i 67 Now consider the laminate created by removing the cracked plies and joining the remaining plies; call it the uncracked laminate. By laminated plate analysis of the symmetric uncracked laminate Tsai, 987, it can be shown that i= i= v i Q i i= v i α xxq i i + αi yy Q i v i α xxq i i + αi yy Q i kj = Au kj = B = B B A u αu xx + A u αu yy A u αu xx + A u αu yy / ol. 64, DECEMBER 997 Transactions of the ASME
10 where A u kj are the elements of the laminated plate theory A] matrix for the uncracked laminate and α xx u and α yy u are the thermal expansion coefficients for the uncracked laminate defined by: α u xx = B α u yy = B a u a u i= i= v i α xxq i i + αi yy Q i + a u v i α xxq i i + αi yy Q i + a u i= i= ] v i α xxq i i + αi yy Q i 7 ] v i α xxq i i + αi yy Q i 7 Here a u kj are elements of the laminated plate theory a] matrix which is the inverse of the A] matrix. Using these results, the effective xdirection thermal expansion coefficient can be expressed as αxx = α xx v + ν xy v 73 where = = B v B v A u A u α xx α xx u α xx α xx u ] + A u α yy α yy u ] + A u α yy α yy u Note that A u kj /B v are the elements of the normalized, x y plane stiffness matrix for the uncracked laminate Tsai, 987. By a similar analysis but with σ 0 applied in the y direction, the effective ydirection thermal expansion coefficient can be expressed as αyy = α yy v Eyy + ν xy v 76 The residual strain energy term is σ r αt = v i σ ir xx α i xxt + v i σ yy ir α yy i T 77 By force balance of residual stresses and isostrain in the uncracked plies σ ir xx σ ir yy v i σ ir xx = 0 and = Q i αxx α xx i = Q i α xx α i xx T + Q i T + Q i Using these results, the residual strain energy term is v i σ ir yy = 0 78 α yy α i yy α yy α i yy T for i 79 T for i 80 σ r αt = constant α xx v T α yy v T 8 The constant term is not evaluated because it drops out when finding the energy release rate. Substituting Eqs. 5, 73, 76, and 8 into Eq. 5 gives G = d d ν xy σ 0 v T + v T σ 0 v T ] + v T d 8 E yy Journal of Applied Mechanics ol. 64, DECEMBER 997 / 83
11 The energy release rate depends only on, Eyy, and νxy, all of which can be evaluated by an isothermal stress analysis. Equation 8 is exact for any damage mode in a microcracked laminate. If the damage is mode I propagation of a new microcrack between the existing microcracks, we can use Eq. 3 to derive an exact relation between laminate effective properties: d d ν xy E xx = d d E yy ν 83 xy Interestingly, an analysis of fracture in the presence of residual thermal stresses has lead to a relation between effective mechanical properties. Using Eq. 83 the mode I microcracking energy release is G I = σ 0 v T d d E xx E xx + v T d ν ] xy 84 The mode I energy release rate depends only on and νxy. McCartney 994 derived results that appear equivalent to Eqs. 8 and 83. McCartney s results, however, were a specific result of an approximate generalized, planestrain, thermal elasticity analysis of a microcracked laminate. The results here were derived by a very different path and are exact provided exact results for, νxy, and Eyy are known. The previous results were for uniaxial loading. It is trivial to extend the analysis to generalized inplane loading of the microcracked laminate. The energy release rate becomes G = d E ν xy xx E 0 xx Note: / is a σeff ν xy Eyy 0 σ eff correction vs published paper G xy where G xy is the effective inplane shear modulus and σ eff is the effective inplane applied stressed defined by σ eff = σ x0 v T, σ y0 v T, τ xy0 86 Here σ x0, σ y0, and τ xy0 are the applied inplane stresses. Discussion In many examples considered, the energy release rate for crack growth, G, was reduced to an expression that depends only on the effective compliance S or stiffness C tensors and the phase average mechanical stresses. Because these terms can be evaluated by isothermal elasticity methods Hashin 963; 969, it is often possible to include the effect of residual thermal stresses on the energy release rate without ever evaluating the thermal stresses. In other words, no thermal elasticity analysis of the composite is required. This result, however, does not imply that the effect of residual thermal stresses is a trivial extension of isothermal fracture mechanics analysis. For example, the isothermal energy release rate for microcracking of a laminate depends only on the. In contrast, the energy release rate in the presence of residual stresses depends on, νxy, and Eyy. Thus, in general, the fracture mechanics analysis of a composite with residual thermal stresses will require more isothermal elasticity analysis of composite properties than the corresponding isothermal fracture mechanics analysis. The discussion here was confined to residual thermal stresses, but identical results could be derived for other types of residual stresses. For example, fiberreinforced, polymermatrix composites can develop residual stresses due to differential moisture absorption between the fibers and the matrix Tsai, 987. The results for moistureinduced residual stresses can be generated from the results given here by replacing α by the moisture expansion tensor and T by the moisture concentration. Residual stresses induced by nonuniform 84 / ol. 64, DECEMBER 997 Transactions of the ASME
12 temperature T a function of position are more complicated. The general theory derived here up to Eq. 3 still applies when there is nonuniform T. Many subsequent simplifications, however, only hold for uniform T. The energy release rate in the presence of residual stresses depends on derivatives of mechanical terms like ds, dc, and dσ im 87 Many damage mechanics models have been developed that give effective properties as a function damage. The results in this paper could easily be incorporated into such models to simultaneously give the energy release rate for damage growth. An important observation, however, is that the ability of a damage analysis to predict effective properties is necessary but not sufficient justification for use of that analysis to calculate energy release rate. The problem is that calculating derivatives of effective properties is a harder problem than calculating the average property itself. Analyses that are accurate to within a few percent for effective properties may be grossly in error when calculating the derivative. Thus any damage mechanics analysis that seeks to calculate energy release rate must be verified to have accurate derivatives of the required terms. Experimentally this verification can be done by comparing fracture experiments to fracture mechanics predictions. In contrast, experimental verification based on effective property predictions, such as modulus reductions, are inadequate tests of energy release rate models. Acknowledgments This work was supported, in part, by a grant from the Mechanics of Materials program at NSF CMS , and, in part, under McDonnell Douglas contract NAMP References Aboudi, J., 994, Interfacial Damage, Damage Mechanics of Composite Materials, ed., Ramesh Talreja, Elsevier, Amsterdam, pp Charalambides, M., A. J. Kinloch, Y. Wang, and J. G. Williams, 99, On the Analysis of MixedMode Failure, Int. J. Fract., ol. 54, pp Hashemi, S., Kinloch, A. J., and Williams, J. G., 990, The Analysis of Interlaminar Fracture in Uniaxial Fibre Reinforced Polymer Composites, Proc. R. Soc. Lond., ol. A347, pp Hashin, Z., 963, Theory of Mechanical Behavior of Heterogeneous Media, Applied Mechanics Reviews, ol. 7, pp. 9. Hashin, Z., 969, Theory of Composite Materials, Mechanics of Composite Materials, Pergamon Press, pp Hashin, Z., 988, Thermal Expansion Coefficients of Cracked Laminates, Comp. Sci. & Tech., ol. 3, pp Hill, R., 963, Elastic Properties of Reinforced Solids: Some Theoretical Principles, J. Mech. Phys. Solids, ol., pp Levin,. M., 967, On the Coefficients of Thermal Expansion in Heterogeneous Materials, Mechanics of Solids, ol., pp McCartney, L. N., 994, The Prediction of NonUniform Cracking in Biaxially Loaded CrossPly Laminates, National Physical Laboratory, Teddington, United Kingdom, Report DMMA 4. Nairn, J. A., Hu, S., and Bark, J. S., 993, A Critical Evaluation of Theories for Predicting Microcracking in Composite Laminates, J. Mat. Sci., ol. 8, pp Nairn, J. A., and Hu, S., 994, Micromechanics of Damage: A Case Study of Matrix Microcracking, Damage Mechanics of Composite Materials, ed., Ramesh Talreja, Elsevier, Amsterdam, pp Nairn, J. A., 995, Some New ariational Mechanics Results on Composite Microcracking, Proc. 0 th Int l Conf. on Comp. Mat., ol. I, pp Rosen, B. W., and Hashin, Z., 970, Effective Thermal Expansion Coefficients and Specific Heats of Composite Materials, Int. J. Engng. Sci., ol. 8, pp Tsai, T. W., 987, Composites Design, Think Composites, Dayton, Ohio. Journal of Applied Mechanics ol. 64, DECEMBER 997 / 85
FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT INTERFACES, AND TRACTIONLOADED CRACKS
Composites Science and Technology, 61, 159167 (000) c 000 Elsevier Science Limited Author Prepared Preprint. All rights reserved ELSEVIER FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES
Advanced Composite Letters, Vol. 9, No. 6, 373383 000 Full Article ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES John A. Nairn Material
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMicrocracking, MicrocrackInduced. Delamination, and Longitudinal
NASA Contractor Final Report Microcracking, MicrocrackInduced Delamination, and Longitudinal Splitting of Advanced Composite Structures John A. Nairn University of Utah Salt Lake City, Utah Prepared for
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationFracture Mechanics Analysis of Composite Microcracking: Experimental Results in Fatigue
Proceedings of the 5 th Technical Conference on Composite Materials, American Society of Composites, East Lansing, Michigan, June 1114, 1990). Fracture Mechanics Analysis of Composite Microcracking: Experimental
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationThe Initiation and Growth of Delaminations Induced by Matrix Microcracks in Laminated Composites
International Journal of Fracture, 57, 1 4 199. The Initiation and Growth of Delaminations Induced by Matri Microcracks in aminated Composites J. A. NAIRN and S. HU Department of Materials Science and
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationFracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach Ludovic Noels Computational & Multiscale Mechanics of
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationA MULTISCALE DAMAGE MODEL FOR THE ANALYSIS OF LAMINATED COMPOSITE STRUCTURES ON THE MICROSCALE
A MULTISCALE DAMAGE MODEL FOR THE ANALYSIS OF LAMINATED COMPOSITE STRUCTURES ON THE MICROSCALE P. Ladevèze 1,2, M. Trovalet 1, G. Lubineau 1 1 LMTCachan (ENS Cachan/CNRS/UPMC/Pres Universud Paris) 61
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationOn the calculation of energy release rates for cracked laminates with residual stresses
International Journal of Fracture, 39, 67 93 006) On the calculation of energy release rates for cracked laminates with residual stresses J. A. NAIRN Wood Science and Engineering, Oregon State University,
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationPredicting Failure of Multiangle Composite Laminates
Predicting Failure of Multiangle Composite Laminates Preliminary discussion (not in textbook): Micromechanics failure analyses vs Macromechanics failure analyses Fiber Architecture of Some Common Composite
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationThe Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries
The Effects of Transverse Shear on the Delamination of EdgeNotch Flexure and 3Point Bend Geometries M. D. Thouless Department of Mechanical Engineering Department of Materials Science & Engineering University
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationINFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK BETWEEN THE TWO LAYERS
Djoković, J. M., et.al.: Influence of Temperature on Behavior of the Interfacial THERMAL SCIENCE: Year 010, Vol. 14, Suppl., pp. S59S68 S59 INFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationCRITERIA FOR MATRIX FAILURE IN CONTINUOUS FRPCOMPOSITES A LITERATURE STUDY. PART II: DELAMINATION
CRITERIA FOR MATRIX FAILURE IN CONTINUOUS FRPCOMPOSITES A LITERATURE STUDY. PART II: DELAMINATION Hannu Lahtinen and Juha Isometsii Rakenteiden Mekaniikka, Vol. 29 No. 1, 1996, s. 2950 ABSTRACT Some
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More information20. Rheology & Linear Elasticity
I Main Topics A Rheology: Macroscopic deformation behavior B Linear elasticity for homogeneous isotropic materials 10/29/18 GG303 1 Viscous (fluid) Behavior http://manoa.hawaii.edu/graduate/content/slidelava
More informationExample 3.7 Consider the undeformed configuration of a solid as shown in Figure 3.60.
162 3. The linear 3D elasticity mathematical model The 3D elasticity model is of great importance, since it is our highest order hierarchical model assuming linear elastic behavior. Therefore, it provides
More informationProject MMS13 Task 5 Report No 3 (M6/D3)
Project MMS13 Task 5 Report No 3 (M6/D3) Material Data Requirements and Recommended Test Methods for the Predictive Modelling of Defect Criticality in Composite Material Systems M R L Gower and G D Sims
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationME 2570 MECHANICS OF MATERIALS
ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationMcMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007
McMAT 2007 Micromechanics of Materials Austin, Texas, June 3 7, 2007 RANDOM POLYCRYSTALS OF GRAINS WITH CRACKS: MODEL OF ELASTIC BEHAVIOR FOR FRACTURED SYSTEMS James G. Berryman Earth Sciences Division
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationCross Laminated Timber Properties Including Effects of NonGlued Edges and Additional Cracks
European Journal of Wood and Wood Products Volume 75, Issue 6, pp 973 983 7) Cross Laminated Timber Properties Including Effects of NonGlued Edges and Additional Cracks John A. Nairn Received: 9 January
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationAccelerated Testing Methodology for Long Term Durability of CFRP
IFREMERONR Workshop on Durability of Composites in a Marine Environment August 23 24, 22 IFREMER Centre, Nantes, France Accelerated esting Methodology for Long erm Durability of CFRP Masayuki Nakada*,
More informationUnderstanding hydraulic fracture variability through a penny shaped crack model for prerupture faults
Penny shaped crack model for prerupture faults Understanding hydraulic fracture variability through a penny shaped crack model for prerupture faults David Cho, Gary F. Margrave, Shawn Maxwell and Mark
More informationNumerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board
Numerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board John A. Nairn (Professor) and Edward Le (PhD Student) Wood Science & Engineering,
More informationLinear Elastic Fracture Mechanics
Measure what is measurable, and make measurable what is not so.  Galileo GALILEI Linear Elastic Fracture Mechanics Krishnaswamy RaviChandar Lecture presented at the University of Pierre and Marie Curie
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationStress intensity factor analysis for an interface crack between dissimilar isotropic materials
Stress intensity factor analysis for an interface crack between dissimilar isotropic materials under thermal stress T. Ikeda* & C. T. Sun* I Chemical Engineering Group, Department of Materials Process
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationMECHANICS OF COMPOSITE STRUCTURES
MECHANICS OF COMPOSITE STRUCTURES LÁSZLÓ P. KOLLÁR Budapest University of Technology and Economics GEORGE S. SPRINGER Stanford University PUBLISHED BY THE PRESS SYNDICATE OF THE UNIVERSITY OF CAMBRIDGE
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationTentamen/Examination TMHL61
Avd Hållfasthetslära, IKP, Linköpings Universitet Tentamen/Examination TMHL61 Tentamen i Skademekanik och livslängdsanalys TMHL61 lördagen den 14/10 2000, kl 812 Solid Mechanics, IKP, Linköping University
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More information1 Durability assessment of composite structures
1 Durability assessment of composite structures 1.1 Introduction Composite structures for mechanical and aerospace applications are designed to retain structural integrity and remain durable for the intended
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationNumerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model
Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive Zone Model Numerical Simulation of the Mode I Fracture of Angleply Composites Using the Exponential Cohesive
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationLecture M1 Slender (one dimensional) Structures Reading: Crandall, Dahl and Lardner 3.1, 7.2
Lecture M1 Slender (one dimensional) Structures Reading: Crandall, Dahl and Lardner 3.1, 7.2 This semester we are going to utilize the principles we learnt last semester (i.e the 3 great principles and
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More information